General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.84 - 7.85 g/cm³ Show Material materials with Density of 7.84 - 7.85 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa | |

20.0 °C | 212 GPa Show Material materials with Elastic modulus of 212 GPa | ||

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | ||

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | ||

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | ||

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | ||

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | ||

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | ||

Elongation | 20.0 °C | 22 - 24 % Show Material materials with Elongation of 22 - 24 % | |

Poisson's ratio | 23.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | Typical for Low Carbon Steel |

Shear modulus | 23.0 °C | 82 GPa Show Material materials with Shear modulus of 82 GPa | Typical for Low Carbon Steel |

Tensile strength | 20.0 °C | 340 - 510 MPa Show Material materials with Tensile strength of 340 - 510 MPa | |

Yield strength | 20.0 °C | 215 - 275 MPa Show Material materials with Yield strength of 215 - 275 MPa | |

Yield strength Rp0.2 | 50.0 °C | 205 - 266 MPa Show Material materials with Yield strength Rp0.2 of 205 - 266 MPa | |

100.0 °C | 196 - 250 MPa Show Material materials with Yield strength Rp0.2 of 196 - 250 MPa | ||

150.0 °C | 176 - 232 MPa Show Material materials with Yield strength Rp0.2 of 176 - 232 MPa | ||

200.0 °C | 157 - 213 MPa Show Material materials with Yield strength Rp0.2 of 157 - 213 MPa | ||

250.0 °C | 137 - 195 MPa Show Material materials with Yield strength Rp0.2 of 137 - 195 MPa | ||

300.0 °C | 108 - 179 MPa Show Material materials with Yield strength Rp0.2 of 108 - 179 MPa | ||

350.0 °C | 88 - 166 MPa Show Material materials with Yield strength Rp0.2 of 88 - 166 MPa | ||

400.0 °C | 68 - 156 MPa Show Material materials with Yield strength Rp0.2 of 68 - 156 MPa | ||

Unlock all property charts |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | |

20.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

100.0 °C | 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.25E-5 1/K | ||

200.0 °C | 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.3E-5 1/K | ||

300.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | ||

400.0 °C | 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.41E-5 1/K | ||

500.0 °C | 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 1/K | ||

600.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | ||

Unlock all property charts | |||

Max service temperature | 500 °C Show Material materials with Max service temperature of 500 °C | Typical for Carbon Steel | |

Max service temperature, long | -20 - 400 °C Show Material materials with Max service temperature, long of -20 - 400 °C | ||

Melting point | 1480 - 1526 °C Show Material materials with Melting point of 1480 - 1526 °C | Typical for Low Carbon Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 430 - 461 J/(kg·K) Show Material materials with Specific heat capacity of 430 - 461 J/(kg·K) | ||

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | ||

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | ||

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | ||

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | ||

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | -100.0 °C | 52.6 W/(m·K) Show Material materials with Thermal conductivity of 52.6 W/(m·K) | |

20.0 °C | 53.4 - 54 W/(m·K) Show Material materials with Thermal conductivity of 53.4 - 54 W/(m·K) | ||

100.0 °C | 53.3 W/(m·K) Show Material materials with Thermal conductivity of 53.3 W/(m·K) | ||

200.0 °C | 50.1 W/(m·K) Show Material materials with Thermal conductivity of 50.1 W/(m·K) | ||

300.0 °C | 46.9 W/(m·K) Show Material materials with Thermal conductivity of 46.9 W/(m·K) | ||

400.0 °C | 43.2 W/(m·K) Show Material materials with Thermal conductivity of 43.2 W/(m·K) | ||

500.0 °C | 39.5 W/(m·K) Show Material materials with Thermal conductivity of 39.5 W/(m·K) | ||

600.0 °C | 36.1 W/(m·K) Show Material materials with Thermal conductivity of 36.1 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | -100.0 °C | 18 mm²/s Show Material materials with Thermal diffusivity of 18 mm²/s | |

20.0 °C | 14.8 mm²/s Show Material materials with Thermal diffusivity of 14.8 mm²/s | ||

100.0 °C | 13.7 mm²/s Show Material materials with Thermal diffusivity of 13.7 mm²/s | ||

200.0 °C | 12.1 mm²/s Show Material materials with Thermal diffusivity of 12.1 mm²/s | ||

300.0 °C | 10.6 mm²/s Show Material materials with Thermal diffusivity of 10.6 mm²/s | ||

400.0 °C | 9.2 mm²/s Show Material materials with Thermal diffusivity of 9.2 mm²/s | ||

500.0 °C | 7.6 mm²/s Show Material materials with Thermal diffusivity of 7.6 mm²/s | ||

600.0 °C | 6.1 mm²/s Show Material materials with Thermal diffusivity of 6.1 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | -100.0 °C | 1.3E-7 Ω·m Show Material materials with Electrical resistivity of 1.3E-7 Ω·m |

20.0 °C | 1.95E-7 - 2E-7 Ω·m Show Material materials with Electrical resistivity of 1.95E-7 - 2E-7 Ω·m | |

100.0 °C | 2.4E-7 Ω·m Show Material materials with Electrical resistivity of 2.4E-7 Ω·m | |

200.0 °C | 3.15E-7 Ω·m Show Material materials with Electrical resistivity of 3.15E-7 Ω·m | |

300.0 °C | 4E-7 Ω·m Show Material materials with Electrical resistivity of 4E-7 Ω·m | |

400.0 °C | 5.03E-7 Ω·m Show Material materials with Electrical resistivity of 5.03E-7 Ω·m | |

500.0 °C | 6.26E-7 Ω·m Show Material materials with Electrical resistivity of 6.26E-7 Ω·m | |

600.0 °C | 7.68E-7 Ω·m Show Material materials with Electrical resistivity of 7.68E-7 Ω·m | |

Unlock all property charts |

Magnetic

Property | Value | Comment |
---|---|---|

Curie temperature | 770 °C Show Material materials with Curie temperature of 770 °C | Typical for Low Carbon Steel |

Chemical properties

Property | Value |
---|---|

Aluminium | 0.02 % Show Material materials with Aluminium of 0.02 % |

Carbon | 0.16 % Show Material materials with Carbon of 0.16 % |

Chromium | 0.3 % Show Material materials with Chromium of 0.3 % |

Copper | 0.3 % Show Material materials with Copper of 0.3 % |

Manganese | 0.8 - 1.5 % Show Material materials with Manganese of 0.8 - 1.5 % |

Molybdenum | 0.08 % Show Material materials with Molybdenum of 0.08 % |

Nickel | 0.5 % Show Material materials with Nickel of 0.5 % |

Niobium | 0.05 % Show Material materials with Niobium of 0.05 % |

Nitrogen | 0.01 % Show Material materials with Nitrogen of 0.01 % |

Phosphorus | 0.03 % Show Material materials with Phosphorus of 0.03 % |

Silicon | 0.4 % Show Material materials with Silicon of 0.4 % |

Sulfur | 0.01 - 0.015 % Show Material materials with Sulfur of 0.01 - 0.015 % |

Titanium | 0.03 % Show Material materials with Titanium of 0.03 % |

Vanadium | 0.05 % Show Material materials with Vanadium of 0.05 % |